Cross-linking cellulose nanofibrils for potential elastic cryo-structured gels
© Syverud et al; licensee Springer. 2011
Received: 26 September 2011
Accepted: 12 December 2011
Published: 12 December 2011
Cellulose nanofibrils were produced from P. radiata kraft pulp fibers. The nanofibrillation was facilitated by applying 2,2,6,6-tetramethylpiperidinyl-1-oxyl-mediated oxidation as pretreatment. The oxidized nanofibrils were cross-linked with polyethyleneimine and poly N-isopropylacrylamide-co-allylamine-co-methylenebisacrylamide particles and were frozen to form cryo-structured gels. Samples of the gels were critical-point dried, and the corresponding structures were assessed with scanning electron microscopy. It appears that the aldehyde groups in the oxidized nanofibrils are suitable reaction sites for cross-linking. The cryo-structured materials were spongy, elastic, and thus capable of regaining their shape after a given pressure was released, indicating a successful cross-linking. These novel types of gels are considered potential candidates in biomedical and biotechnological applications.
Keywordscellulose nanofibrils MFC cryogelation cross-linking
The main raw material for the production of microfibrillated cellulose [MFC] is cellulose fibers, produced from wood by chemical pulping. Properly produced MFC contains a major fraction of cellulose nanofibrils . Nanofibrils are composed of bundles of cellulose molecules, arranged in crystalline and amorphous areas. Nanofibrils have threadlike shapes, with diameters in the nanometer scale (< 100 nm), with high aspect ratio and high specific surface area. The fibrillated material retains many of the advantageous properties of cellulose fibers, such as high strength and the ability to self-assemble by making strong inter-fibril bonds. The small dimensions and the large specific surface area open up for applications that may not yet be foreseen. Several recent publications demonstrate how the strength properties of cellulose nanofibrils can be utilized for various purposes, e.g., in nanocomposites [1–6], to improve strength properties of paper [7, 8], in thin films with high strength  and with added functionality such as antimicrobial activity .
Nanofibrils have hydroxyl groups on their surfaces, which can be used as targets for surface modification. Pretreatment of cellulose fibers with 2,2,6,6-tetramethylpiperidinyl-1-oxyl [TEMPO] prior to fibrillation introduces carboxylic acid groups and small amounts of aldehyde groups (0.2 to 0.3 mmol/g) , which can react easily with amines .
Subjecting a solution or suspension to temperatures below the freezing point but above the eutectic point of the system leads to the formation of a two-phase system, with one solid and one liquid phase. When ice crystals form, any solutes or particles are expelled into a non-frozen phase, which forms around the crystals. In cryogelation, the gelation process occurs in the non-frozen phase, and hence, a material is formed under apparently frozen conditions . The gelation can either occur through chemical cross-linking, polymerization reactions, or through non-covalent interactions. However, it is crucial that the interactions do not reverse when the sample thaws since that would make it impossible to form a material through cryogelation. Thawing the sample results in melting of the ice crystals while the material, formed through gelation, retains its shape. A macroporous material can thus be formed, in which the pores are a replica of the ice crystals .
Pores in materials formed through cryogelation are interconnected and normally exhibit diameters between 1 and 100 μm, depending on freezing temperatures and composition of the starting mixture. Cryogelation does not require a freeze-drying step in order to produce a macroporous structure. The technique is only based on a freeze-thawing process. Cryogels are highly macroporous and often elastic materials, which can make them suitable in applications where traditional hydrogels would not be applicable. These gels have been used for biotechnological applications such as chromatography materials to process particle-containing fluids or enzyme immobilization . Within biomedical applications, cryogels are being used in scaffolds for the cultivation of mammalian cells in tissue engineering applications .
The application of cellulose nanofibrils as a main component, in combination with polymers/particles as cross-linkers to form macroporous hydrogels, has not been investigated yet. It is expected that such gels can have a major potential within, e.g., biomedical applications. This study thus focuses on the ability of cellulose nanofibrils combined with cryogelation to produce cryo-structured gels with elastic properties. Two different routes will be applied for cross-linking, i.e., reactions with polyethyleneimine [PEI] and poly N-isopropylacrylamide-co-allylamine-co-methylenebisacrylamide [pNIPA] particles.
Production of cellulose nanofibrils
Two series of nanofibril qualities were produced from 100% P. radiata kraft pulp fibers. One of the series was chemically pretreated by using TEMPO-mediated oxidation, according to Saito et al. . The other series was homogenized without pretreatment. The fibers were homogenized with a Rannie 15 type 12.56X homogenizer operated at 1,000 bar pressure. The pulp consistency during homogenizing was 0.5%. Samples of the fibrillated materials were collected after five passes through the homogenizer. For details, see the work of Syverud et al. .
The nanofibrillated material had a concentration of approximately 0.5% (w/v). PEI (0.4% w/v; molecular weights 600 and 1,800 g/mol) from PolyScience (Niles, IL, USA) was added to this suspension. This mixture was thereafter frozen at -12°C and stored for 16 h; after which, the samples were thawed at room temperature, and the obtained gels were washed with water.
The second route for preparing gels consisted the adding of pNIPA particles (0.04% w/v)  to the nanofibril suspension. Allylamine and N,N'-methylene-bisacrylamide were purchased from Sigma-Aldrich (Steinheim, Germany), and N-isopropylacrylamide was from Acros (Geel, Belgium). The mixture was thereafter frozen at -12°C and stored for 16 h. The samples were then thawed at room temperature, and the obtained gels were washed with water.
The prepared samples were cut into a 2-mm-thin disc and fixed in 2.5% w/v glutaraldehyde in 0.1 M sodium phosphate buffer (pH 7.4) overnight at +4°C. The samples were thereafter stepwise dehydrated in ethanol (0%, 25%, 50%, 75%, 96%, 99.6%) and then critical-point dried. The dried samples were sputter-coated with gold/palladium (40/60) and examined using a JEOL JSM-5000LV scanning electron microscope [SEM] (JEOL Ltd., Akishima, Tokyo, Japan). In addition, the cross-linked nanostructures were freeze-dried and assessed with a Zeiss Ultra field-emission scanning electron microscope [FESEM] (Carl Zeiss AG, Oberkochen, Germany) at various magnifications.
The mechanical stability of the cryo-structured gels was assessed using a texture analyzer (XT2i, Stable Micro Systems, Godalming, England), using a 5-kg load cell and a cylindrical probe (25 mm in diameter).
Results and discussion
The results presented in this study indicate that the nanofibrils are interesting building blocks to prepare cryo-structured materials. Based on the sponge-like property of these cryo-structured materials, we foresee high-tech applications, such as modified macroporous structures in biomedical and biotechnology areas.
Oxidized nanofibrils, produced from P. radiata pulp fibers, were cross-linked with PEI and pNIPA particles in order to form cryo-structured gels. Due to a successful cross-linking, the nanofibrils formed stable 3-D networks. The cryo-structured materials were spongy, elastic, and thus capable of regaining their shape after a given pressure was released. Such characteristics propose the cryo-structured nanomaterials as most promising within biomedicine and biotechnology applications.
field emission scanning electron microscope
lower critical solution temperature
scanning electron microscope.
The work was partly financed by the Research Council of Norway through the grant, 196119/V30.
- Chinga-Carrasco G: Cellulose fibres, nanofibrils and microfibrils: the morphological sequence of MFC components from a plant physiology and fibre technology point of view. Nanoscale Res Lett 2011, 6: 417.View Article
- Henriksson M, Berglund L: Structure and properties of cellulose nanocomposite films containing melamine formaldehyde. J Appl Polym Sci 2007, 106: 2817–2824.View Article
- Nakagaito AN, Yano H: Novel high-strength biocomposites based on microfibrillated cellulose having nano-order-unit web-like network structure. Appl Phys A 2005, 80: 155–159.View Article
- Bruce DM, Hobson RN, Farrent JW, Hepworth DG: High-performance composites from low-cost plant primary cell walls. Compos Part A 2005, 26: 1486–1493.View Article
- Malainine ME, Mahrouz M, Dufresne A: Thermoplastic nanocomposites based on cellulose microfibrils from Opuntia ficus-indica parenchyma cell. Compos Sci Technol 2005, 65: 1520–1526.View Article
- López-Rubio A, Lagaron JM, Ankerfors M, Lindström T, Nordqvist D, Mattozzi A, Hedenqvist MS: Enhanced film forming and film properties of amylopectin using micro-fibrillated cellulose. Carbohydr Polym 2007, 68: 718–727.View Article
- Eriksen Ø, Gregersen ØW, Syverud K: The use of microfibrillated cellulose produced from kraft pulp as strength enhancer in TMP pulp. Nordic Pulp Pap Res J 2008, 23: 299–304.View Article
- Mörseburg K, Chinga-Carrasco G: Assessing the combined benefits of clay and nanofibrillated cellulose in layered TMP-based sheets. Cellulose 2009, 16: 795–806.View Article
- Syverud K, Stenius P: Strength and barrier of MFC films. Cellulose 2009, 16: 75–85.View Article
- Andresen M, Stenstad P, Møretrø T, Langsrud S, Syverud K, Johansson L-S, Stenius P: Nonleaching antimicrobial films prepared from surface-modified microfibrillated cellulose. Biomacromolecules 2007, 8: 2149–2155.View Article
- Saito T, Nishiyama Y, Putaux J-L, Vignon M, Isogai A: Homogeneous suspensions of individualized microfibrils from TEMPO-catalyzed oxidation of native cellulose. Biomacromolecules 2006, 7: 1687–1691.View Article
- Montgomery MW, Day EA: Aldehyde-amine condensation reaction: a possible fate of carbonyls in foods. J Food Sci 1965, 30: 828–832.View Article
- Lozinsky VI: Cryogels on the basis of natural and synthetic polymers: preparation, properties and application. Russ Chem Rev 2002, 71: 489–511.View Article
- Arvidsson P, Plieva FM, Lozinsky VI, Galaev IY, Mattiasson B: Direct chromatographic capture of enzyme from crude homogenate using immobilized metal affinity chromatography on a continuous supermacroporous adsorbent. J Chromatogr A 2003, 986: 275–290.View Article
- Bölgen N, Plieva F, Galaev IY, Mattiasson B, Piskin E: Cryogelation for preparation of novel biodegradable tissue-engineering scaffolds. J Biomater Sci Polym Ed 2007, 18: 1165–1179.View Article
- Syverud K, Chinga-Carrasco G, Toledo J, Toledo P: A comparative study of Eucalyptus and Pinus radiata pulp fibres as raw materials for production of cellulose nanofibrils. Carb Pol 2010, 84: 1033–1038.View Article
- Hajizadeh S, Kirsebom H, Mattiasson B: Characterization of macroporous carbon-cryostructured particle gel, an adsorbent for small organic molecules. Soft Matter 2010, 6: 5562–5569.View Article
- Kirsebom H, Mattiasson B, Galaev IY: Ultrafast responsive poly(N-isopropylacrylamide) gel produced by cryostructuring of self-crosslinkable polymer microgels. Macromol Rapid Commun 2010, 31: 1095–1100.View Article
- Zhang X-Z, Yang Y-Y, Chung T-S, Ma K-X: Preparation and characterization of fast response macroporous poly(N-isopropylacrylamide) hydrogels. Langmuir 2001, 17: 6094–6099.View Article
- Chinga-Carrasco G, Yu Y, Diserud O: Quantitative electron microscopy of cellulose nanofibril structures from Eucalyptus and Pinus radiata kraft pulp fibres. Microsc microanal 2011, 17: 563–571.View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.